Materials 2015, 8, 5479-5489; doi:10.3390/ma8085260
materials ISSN 1996-1944 www.mdpi.com/journal/materials Article
Recyclability of Concrete Pavement Incorporating High Volume of Fly Ash Isamu Yoshitake 1, *, Takeo Ishida 2,: and Sunao Fukumoto 3 1
Department of Civil and Environmental Engineering, Yamaguchi University, Tokiwadai 2-16-1, Ube, Yamaguchi 755-8611, Japan 2 Cement and Construction Materials Company, Ube Industries, Ogushi Okinoyama 1-6, Ube, Yamaguchi 755-8633, Japan; E-Mail: [email protected]
3 The Chugoku Electric Power Co. Inc., Komachi 4-33, Naka-ku, Hiroshima, Hiroshima 730-8701, Japan; E-Mail: [email protected]
These authors contributed equally to this work.
* Author to whom correspondence should be addressed; E-Mail: [email protected]
; Tel.: +81-836-85-9306; Fax: +81-836-85-9301. Academic Editor: Prabir K. Sarker Received: 27 July 2015 / Accepted: 17 August 2015 / Published: 21 August 2015
Abstract: Recyclable concrete pavement was made from fly ash and crushed limestone sand and gravel as aggregates so that the concrete pavement could be recycled to raw materials for cement production. With the aim to use as much fly ash as possible for the sustainable development of society, while achieving adequate strength development, pavement concrete having a cement-replacement ratio of 40% by mass was experimentally investigated, focusing on the strength development at an early age. Limestone powder was added to improve the early strength; flexural strength at two days reached 3.5 MPa, the minimum strength for traffic service in Japan. The matured fly ash concrete made with a cement content of 200 kg/m3 achieved a flexural strength almost equal to that of the control concrete without fly ash. Additionally, Portland cement made from the tested fly ash concrete was tested to confirm recyclability, with the cement quality meeting the Japanese classification of ordinary Portland cement. Limestone-based recyclable fly ash concrete pavement is, thus, a preferred material in terms of sustainability. Keywords: fly ash; recyclability; cement; concrete pavement; limestone; early strength
Materials 2015, 8
1. Introduction Asphalt concrete pavement accounts for approximately 95% of the total length of road in Japan. Cement concrete pavement accounts for less than 5% of the total length because of the concerns of construction costs and traffic noise, yet it has adequate durability and superior life-cycle cost. Most concrete pavement requires a relatively long curing term before traffic service, which negatively affects its use as a pavement material. Fly ash collected from coal-burning power plants has remarkable properties that can improve the performance of cement concrete when added, and the powder material is, thus, often used as a supplemental binder of Portland cement in concrete (fly ash concrete). The greatest concern about fly ash concrete is the gradual strength development at an early age. Thus, when fly ash concrete is employed as a pavement material, the traffic service must be further delayed. Limestone powder can be added to improve strength development via the micro-filler effect and help accelerate the reaction at an early age. Bentz et al.  reported the properties of high-volume fly ash (HVFA) mixtures enhanced with the addition of limestone powder. Bentz et al.  used limestone powder with a particle size of up to five micrometers as a cement-replacement material for HVFA concrete and found that the early-age reaction was accelerated by replacing 5% of the cement volume with limestone powder. Yoshitake et al. [3,4] examined the tensile properties of HVFA concrete made with limestone aggregate and powder. In particular, they presented the uniaxial tensile strength and tensile Young’s modulus of the HVFA concrete. In addition, they addressed the possibility of recyclable concrete for cement production. Fundamental properties and applications of HVFA concrete were summarized in high-performance and high-volume fly ash concrete . Additionally, applications for road pavement have been introduced in the literature on HVFA concrete. Das  examined various properties of fresh and hardened HVFA concrete applicable for road pavement. That study investigated the design of rigid pavement using the HVFA concrete and compared the cost performance with that of conventional concrete pavement. Naik et al.  reported the mechanical properties and durability of HVFA concrete pavement incorporating classes C and F of fly ash. In addition, Naik et al.  conducted a field study to investigate the long-term performance of concrete pavements made with a high volume of class-C and -F fly ash. They described long-term performances (ages of 7 to 14 years) and reported that long-term compressive strengths of class-F fly ash concretes were better than those of Class-C fly ash concretes. Atis and Celik  investigated the relations between abrasion resistance and compressive/flexural strengths of pavement concrete made with a high volume of class-F fly ash. They presented a strong linear relation between abrasion resistance and flexural strength. Atis  examined the strength properties of roller-compacted and workable HVFA concretes having cement replacement ratios of 50% and 70%. According to their investigation, the HVFA concrete had higher compressive and tensile strengths than normal concrete made without fly ash. They concluded that HVFA concrete is an adequate material for both structural and pavement applications. Kumar et al.  performed a laboratory test to examine compressive and flexural strengths of pavement concretes. The tested concretes were made with three water-cementitious material ratios (w/cm = 0.40, 0.34, 0.30) and 20%–60% cement replacement by fly ash. The test results showed that the concrete containing 40% fly ash developed the maximum strength. Rashad et al.  prepared HVFA concretes blended with silica fume and granulated blast-furnace slag,
Materials 2015, 8
and conducted compression and abrasion tests. They reported that concrete containing 50% fly ash, 10% silica fume and 10% granulated blast-furnace slag had the maximum compressive strength among the HVFA concrete specimens. Nassar et al.  reported a field investigation of HVFA concrete pavement, including strength of concrete cores at the age of 270 days and abrasion resistance. They addressed that HVFA concrete can contribute economic construction and improve the service life of the infrastructure. According to the definition of HVFA concrete , fly ash is used as a cementitious material to replace 50% or more of the cement by mass. A concern about HVFA concrete is the strength development at an early age, while HVFA concrete has numerous advantages for structural application. Concrete pavement often requires an adequate early strength for practical use, and the strength development should thus be improved. The present study aims to develop a fly ash concrete pavement having adequate strength at an early age. The ratio of cement replacement by fly ash was designed as 40% (FA/cm = 0.4) by referring to previous investigations [7,11]. To improve the strength development at an early age, limestone powder was added to the fly ash concrete. Furthermore, crushed limestone was used as all fine and coarse aggregates in the concrete following previous studies [3,4]. Concrete made with limestone aggregate has a remarkably low coefficient of thermal expansion, which reduces thermal cracking in concrete pavement. It is of interest that all components of the concrete are materials that can be used in manufacturing Portland cement [14,15]. In particular, the recycling of the concrete is relatively feasible because steel-reinforcement is seldom used in most concrete pavements. The present study focuses on developing a recyclable fly ash concrete pavement having adequate early strength and confirming the recyclability for cement production. This paper presents fundamental properties of the recycled cement made from the fly ash concrete pavement. 2. Flexural Strength 2.1. Materials Table 1 summarizes fundamental properties of the materials used in this study. Fine and coarse aggregates used in the concrete were crushed limestone sand (2.62 g/cm3 ) and crushed limestone (2.68 g/cm3 ) so as to ensure the recyclability for cement production. To eliminate the influence of temperature on the fresh properties of concrete, all materials had been stored in a temperature-controlling room (20 ˝ C) for 24 h or more. Powder materials in the recyclable concrete were ordinary Portland cement, limestone powder and fly ash. Table 2 gives chemical compositions of the cement and limestone powder. The limestone powder was added to improve strength development at an early age. A type-II fly ash as defined by Japanese standards  was used in the study; the fly ash has properties similar to those of class-F fly ash in ASTM C618 . Table 3 gives the properties and chemical composition of the fly ash. A high-range water-reducing admixture (HRWRA) was used to obtain an appropriate slump (20 mm) for the pavement concrete made with a very low water-cementitious material ratio (w/cm = 0.33). The HRWRA (1.06 g/cm3 ) used in the study was a commercial air entraining (AE) water-reducing agent of polycarboxylic acid.
Materials 2015, 8
5482 Table 1. Materials used in tests.
Cement (C) Limestone powder (LP) Fly ash (FA) Aggregate Fine aggregate (S) Coarse aggregate (G) Admixture (HRWRA) Admixture (AEA)
Ordinary Portland Cement See Table 2 a Ground limestone powder See Table 2 type II See Table 3 Type Density F.M. b 3 Crushed limestone sand 2.62 g/cm 2.75 Crushed limestone 2.68 g/cm3 N/A c AE water-reducing agent of polycarboxylic acid Air entraining agent for fly ash
Size 5´ mm 20–5 mm
UBE Tancal 200M (Ube Material Ind., Ube, Yamaguchi, Japan); b Fineness modulus; c solid content of 0.6. AE: air entraining.
Table 2. Physical and chemical compositions of cement and limestone powder. Properties Density Blaine fineness Setting time start-end Comp. strength at 3 days at 7 days at 28 days CaO SiO2 Al2 O3 Fe2 O3 MgO SO3 Cl´ ignition loss (ig.loss)
Limestone powder (LP)
3.15 g/cm3 3185 cm2 /g 2 h 19 min–3 h 22 min 28.6 MPa 46.1 MPa 62.5 MPa Chemical Compositions 64.3% 20.4% 5.7% 2.9% 1.08% 1.89% 0.017% 2.25%
2.70 g/cm3 5000 cm2 /g N/A N/A N/A N/A 55.62% 0.09% 0.010% 0.013% 0.35% 0.00% 0.00% 43.8%
Table 3. Properties and chemical compositions of fly ash. Properties Density Blaine fineness pH Chemical Compositions ig.loss SiO2 Al2 O3 Fe2 O3 CaO K2 O MgO SO3 Na2 O
Fly ash (FA) 2.18 g/cm3 3440 cm2 /g 4.6 2.70% 58.2% 23.3% 3.19% 0.98% 1.38% 0.55% 0.24% 0.19%
Materials 2015, 8
2.2. Mixture Proportions Concrete pavement having three mixture proportions were prepared for the experimental study (Table 4). All concretes in this investigation were made with a water-cementitious material ratio of 0.33 and had extremely low consistency, as indicated by an average slump value of 20 mm. The concrete mixture proportions were designed to achieve a specified flexural strength (4.5 MPa) at the age of seven days. It is commonly known that the limestone powder contributes strength development at an early age. The limestone powder was used as a mineral admixture for the pavement concrete. The quantity of limestone powder (50 kg/m3 ) was designed through mixing-tests of fresh concrete. The M-1 mixture was fly ash concrete incorporating limestone powder, while M-2 was fly ash concrete made with more fly ash (40 kg/m3 ) instead of limestone powder. The additional fly ash is regarded for convenience as a mineral admixture like limestone powder. The accurate cementitious material ratios are given in the parenthesis in Table 4. To achieve adequate strength development at an early age, the ratio of cement replacement by fly ash in these two concretes was designed as 0.40 by referring to previous investigations [7,11]. The M-0 concrete was a control mixture without fly ash but including limestone powder. Table 4. Mixture proportions of concrete. Mix. ID
FA/cm a w/cm a W C FA LP S G HRWRA b AEA c
0.0 0.33 110 kg/m3 334 kg/m3 0 kg/m3 50 kg/m3 843 kg/m3 1062 kg/m3 4.68 kg/m3 1.23 kg/m3
0.4 0.33 110 kg/m3 200 kg/m3 134 kg/m3 50 kg/m3 820 kg/m3 1033 kg/m3 4.01 kg/m3 1.20 kg/m3
0.4 (0.47) d 0.33 (0.29) d 110 kg/m3 200 kg/m3 134 + 40 d kg/m3 0 kg/m3 820 kg/m3 1033 kg/m3 3.34 kg/m3 2.00 kg/m3
cementitious material (cement + fly ash); b high-range water-reducing agent; incorporating fly ash as a substitution of limestone powder.
2.3. Test Procedure Thirty concrete beam specimens (100 mm ˆ 100 mm ˆ 400 mm) for each mixture proportion were prepared in a laboratory. All specimens were cured in a temperature-controlled room (20 ˝ C) for 1 day and then stored in a water tank at 20 ˝ C after demolding. To examine the strength development of the pavement concretes, four-point loading tests were conducted at ages of 1, 2, 3, 5, 7, 28, 56, 91, 182 and 364 days. The flexural strength at each test age was taken as the average strength of three beam specimens at the same test age. 2.4. Flexural Strength Figure 1a shows the flexural strength development at an early age (0–7 days). Although both fly ash concretes (M-1 and M-2) had less strength than the control concrete (M-0), the flexural strength
Materials 2015, 8 Materials 2015, 8
development development of of M-1 M-1 was was slightly slightly greater greater than than that that of of M-2 M-2 without without limestone limestone powder. powder. The The observation observation verified the effect of limestone powder (i.e., the micro-filler effect) and the acceleration of the verified the effect of limestone powder (i.e., the micro-filler effect) and the acceleration of the reaction reaction at an early age. Concrete pavement is passable for traffic when the flexural strength is equal to or at an early age. Concrete pavement is passable for traffic when the flexural strength is equalhigher to or than 3.5 MPa . The fly ash concrete M-1 achieved the required strength after two days. Both fly ash higher than 3.5 MPa . The fly ash concrete M-1 achieved the required strength after two days. concretes hadconcretes strength of 4.8 MPa at an4.8 ageMPa of seven reaching the specified Both fly ash hadapproximately strength of approximately at an days, age ofthus seven days, thus reaching strength (4.5 MPa) of most concrete pavement. the specified strength (4.5 MPa) of most concrete pavement. Figure upup to to a concrete ageage of 364 days. A previous test Figure 1b,c 1b,c shows showsthe theflexural flexuralstrength strengthdevelopment development a concrete of 364 days. A previous result   is also shown on the for comparison. The The referenced strength data data werewere recorded in a test result is also shown ongraph the graph for comparison. referenced strength recorded test concretes incorporating class-F fly ashfly(FA/cm = 0.4, =w/cm 0.34). All concretes tested in a on testpavement on pavement concretes incorporating class-F ash (FA/cm 0.4, =w/cm = 0.34). All concretes in the present study had higher than thethan referenced strengthstrength data .data The. difference in strength tested in the present study had strength higher strength the referenced The difference in development was probably due to the different aggregate and water contents of the concrete mixtures. strength development was probably due to the different aggregate and water contents of the concrete Influencing factors of factors flexuralofstrength should be should investigated in detail ininfuture mixtures. Influencing flexuraldevelopment strength development be investigated detail research. in future It is noted Itthat flexural of concrete made from high-early-strength Portland cement achieved research. is the noted that strength the flexural strength of concrete made from high-early-strength Portland the minimum strength after one day under field curing conditions . cement achieved the minimum strength after one day under field curing conditions . Figure 1b,c thethe flexural strengths of theofflythe ashfly concretes M-1 and M-1 M-2 gradually 1b,cshows showsthat that flexural strengths ash concretes and M-2 developed gradually while the strength of the controlof concrete (M-0) concrete hardly increased over 91increased days. It isover noteworthy thatItthe developed while the strength the control (M-0) hardly 91 days. is flexural strengths of fly ash concretes andash M-2 were almost equalM-2 to the strength the control noteworthy that the flexural strengths M-1 of fly concretes M-1 and were almostofequal to the concrete (M-0) after one year. The ultimate strength was higher than the specified strength for common strength of the control concrete (M-0) after one year. The ultimate strength was higher than the pavement concrete,forwhile the concrete incorporated only the 200concrete kg/m3 ofincorporated Portland cement. Thekg/m fly 3ash specified strength common pavement concrete, while only 200 of concrete the present demonstrated adequate development for application as Portland tested cement.in The fly ash study concrete tested in the presentstrength study demonstrated adequate strength pavement concrete. development for application as pavement concrete. M-0
M-2 Flexural strength (MPa)
Flexural strength (MPa)
3.5 3.0 1.5
Flexural strength (MPa)
6.0 4.5 3.0 1.5
4.5 3.0 1.5
84 112 140 168 196 224 252 280 308 336 364
Figure 1. Flexural (a) Early age;(a)(b)Early Linearage; graph;(b) (c) Linear Semi-logarithmic Figure 1. strength Flexuraldevelopment; strength development; graph; (c)graph. Semi-logarithmic graph. 3. Recyclability for Cement Production 3. Recyclability forrecyclability Cement Production To confirm the of the pavement concrete, a Portland cement (recycled cement) was made using test specimens of the fly ash concrete. The age of the concrete specimens was half a year To confirm the recyclability of the pavement concrete, a Portland cement (recycled cement) was made or more. The tested concrete was a raw material for manufacturing cement as an alternative material to using test specimens of the fly ash concrete. The age of the concrete specimens was half a year or more. limestone. The study examined the chemical and physical properties of the recycled cement. The tested concrete was a raw material for manufacturing cement as an alternative material to limestone. The hardened concrete was dried in an oven (105 °C) for 24 h and crushed using a ball mill. The study examined the chemical and physical properties of the recycled cement. Chemical compositions of the concrete were examined employing a Japanese standard test  and X-ray The hardened concrete was dried in an oven (105 ˝ C) for 24 h and crushed using a ball mill. fluorescence analysis. The chemical compositions are summarized in Table 5. Chemical compositions of the concrete were examined employing a Japanese standard test  and X-ray fluorescence analysis. The chemical compositions are summarized in Table 5.
Materials 2015, 8
5485 Table 5. Chemical compositions of the hardened fly ash concrete.
ig.loss SiO2 Al2 O3 Fe2 O3 CaO MgO SO3
39.43% 3.25% 1.05% 0.55% 50.28% 0.47% 0.20%
Na2O K2 O R2 O TiO2 MnO P2 O5 Cl
0.04% 0.07% 0.09% 0.07% 0.02% 0.06% 0.005%
3.1. Cement Clinker A cement clinker, having components similar to those of a reference clinker  given in Table 6, was first produced. The fly ash concrete was used in the clinker as a primary calcium material. The materials used for the recycled cement clinker are summarized in Table 7. Fly ash and siliceous powder were added to control the amount of the silicon component in the cement clinker. Table 6. Mineralogical compositions of the cement clinker and recycled cement. Compositions C3 S C2 S C3 A C4 AF a
Reference Clinker a
56.8% 17.7% 8.9% 8.5%
55.1% 23.1% 9.4% 9.0%
52.9% 21.6% 8.7% 8.9%
reference given in JCA (2007) ; b cement clinker made from the recycled fly-ash concrete.
Table 7. Materials for the cement clinker. Materials
Percentage by Mass
Fly ash concrete Fly ash Siliceous powder Iron oxide (Fe2 O3 ) Gypsum di-hydrate Sodium carbonate (Na2 CO3 ) Potassium carbonate (K2 CO3 )
848.7 kg/t 67.6 kg/t 58.0 kg/t 9.7 kg/t 7.9 kg/t 2.6 kg/t 5.4 kg/t
84.9% 6.76% 5.80% 0.97% 0.79% 0.26% 0.54%
The cement clinker was made with the above materials in an electric furnace. The temperature of the furnace increased from 1000 to 1200 ˝ C over 20 min and from 1200 to 1450 ˝ C over 10 min. The temperature was maintained at 1450 ˝ C for 30 min and then reduced to 1350 ˝ C. Afterward, the clinker was removed from the furnace and quenched to a room temperature of 20 ˝ C. The chemical properties of the cement clinker made from the fly-ash concrete were then examined. The chemical compositions were examined employing the test method given in JIS R5202 . The mineralogical and chemical
Materials 2015, 8
compositions of the cement clinker are summarized in Tables 6 and 8 respectively. The mineralogical compositions were estimated using the Bogue formulae, given as Equations (1)–(5) .
C3 S “ 4.07 ˆ CaO ´ 7.60 ˆ SiO2 ´ 6.72 ˆ Al2 O3 ´ 1.43 ˆ F e2 O3 ´ 2.85 ˆ SO3
C2 S “ 2.87 ˆ SiO2 ´ 0.754 ˆ C3 S
C3 A “ 2.65 ˆ Al2 O3 ´ 1.69 ˆ F e2 O3
C4 AF “ 3.04 ˆ F e2 O3
CaSO4 “ 1.70 ˆ SO3
Table 8. Chemical compositions of the cement clinker and recycled cement. Compositions
JIS R 5210 (2009) a
ig.loss SiO2 Al2 O3 Fe2 O3 CaO MgO SO3 Na2 O K2 O R2 O TiO2 MnO P2 O5 Cl
0.12% 22.52% 5.42% 2.96% 66.04% 0.83% 0.67% 0.32% 0.48% 0.64% 0.29% 0.05% 0.16% N/A
1.21% 21.45% 5.16% 2.93% 64.41% 0.79% 2.57% 0.31% 0.52% 0.65% 0.27% 0.05% 0.15% 0.00%